Multilayers of InGaAs Nanostructures Grown on GaAs(210) Substrates
© The Author(s) 2010
Received: 4 March 2010
Accepted: 10 May 2010
Published: 27 May 2010
Multilayers of InGaAs nanostructures are grown on GaAs(210) by molecular beam epitaxy. With reducing the thickness of GaAs interlayer spacer, a transition from InGaAs quantum dashes to arrow-like nanostructures is observed by atomic force microscopy. Photoluminescence measurements reveal all the samples of different spacers with good optical properties. By adjusting the InGaAs coverage, both one-dimensional and two-dimensional lateral ordering of InGaAs/GaAs(210) nanostructures are achieved.
KeywordsMolecular beam epitaxy InGaAs nanostructures GaAs(210) Lateral ordering
On GaAs(100), the extensively investigated surface orientation, the InGaAs growth proceeds in a fashion of two-dimensional (2D) layering plus nanoscale 3D islanding, as driven by strain elastic relaxation due to sufficient lattice mismatch. The resulted 3D islands buried in the GaAs matrix, so-called quantum dots (QDs), have attracted a lot of attentions in the field of the compound semiconductor research in the last 15 years, for their rich spectrum of optoelectronic applications [1–4]. On the other hand, on GaAs(110), another important low index surface orientation, the InGaAs growth proceeds in a layer-by-layer 2D mode without introducing 3D islands [5, 6]. The accumulating strain is expected to be relaxed in a later stage through introducing misfit dislocations. Since (110) is the natural cleaved face of GaAs substrates, the unique growth mechanism leads to cleaved-edge overgrowth of aligned InGaAs QDs through incorporated Al content into the underlying growth base [7, 8].
The InGaAs growth on GaAs high-index substrates orientated between (100) and (110) is still a mystery. On the other hand, other high-index surfaces, especially GaAs(n11), have received significant attention and hosted wide range of InGaAs nanostructures with distinguished functions. For example, InGaAs quantum wires are observed on GaAs(311)A and a unique growth mode is revealed, starting from 2D, through 1D, and finally leading to 3D . Most recently, a remarkable achievement is the ability to tune both vertical and lateral alignments of QDs in InGaAs multilayers on GaAs(n11)B .
GaAs(210) is a plane located in between (100) and (110), 26.6° away from (100) and 18.4° away from (110). In this letter, we reveal the growth phenomena of InGaAs multilayers on GaAs(210) and demonstrate lateral ordered arrays of both quantum dashes and quantum wires.
All samples presented in this study were grown using solid source Molecular Beam Epitaxy (MBE) 32P Riber system. After growth of 0.5-μm-thick GaAs buffer layer at 580°C with a growth rate of 1 monolayer per second (ML/s) under a constant As beam equivalent pressure of 1 × 10−5 Torr, 15.5 periods multilayered In0.4Ga0.6As/GaAs structures of different GaAs spacer layer thicknesses or of different In0.4Ga0.6As coverages were grown. Three samples of different spacers at 120, 70, and 50 ML respectively have the same In0.4Ga0.6As coverage of 7 ML. One additional sample of 70 ML spacer has the In0.4Ga0.6As coverage of 5.7 ML. The growth of In0.4Ga0.6As layer was performed at 540°C and As beam equivalent pressure of 4.4 × 10−6 Torr. After growth of first 5 ML of GaAs spacer at 540°C, the temperature of growth was rapidly increased up to 580°C, and As beam equivalent pressure was turned back to 1 × 10−5 Torr. The quality of growth and growth rates were monitored by RHEED. All growths were ended by In0.4Ga0.6As layer for following atomic force microscopy (AFM) studies. For optical properties of the samples, the photoluminescence (PL) measurements were performed in a variable temperature 10–300 K closed-cycle helium cryostat. The 532-nm line from a Nd:YAG (yttrium aluminum garnet) laser was used for continuous-wave (CW) PL excitation. The laser spot diameter was about 20 μm and the optical excitation power was in the range of 10−6–102 mW. The PL signal from the sample was dispersed by a 0.5-m single-grating monochromator and detected by liquid nitrogen (LN)-cooled InGaAs photodiode detector array.
The AFM data in Fig. 1 suggest a structural coupling and the PL data in Fig. 2 indicate an electronic coupling between subsequent InGaAs layers. Since the growth mechanism has been well documented [13, 14], vertical alignments of InGaAs nanostructures as a result of strain field interaction among subsequent layers are expected. With reducing the spacer thickness, more strain fields transmitted to the following layer; therefore, the growth proceeds in a more efficient approach to relax the accumulating strain. As the result, the quantum dashes become shorter and a transition to arrow-like nanostructures is observed.
In conclusion, the nanostructure evolution of InGaAs/GaAs multilayers along (210) is investigated. 2D-ordered quantum dashes and uniformly spaced quantum wires are observed. The results are explained in terms of strain-driven mechanism with considering the amount of strain build-up. Such a report of InGaAs nanostructures on a surface index between (100) and (110) could help to achieve a comprehensive understanding of strain-driven growth in general.
This article is distributed under the terms of the Creative Commons Attribution Noncommercial License which permits any noncommercial use, distribution, and reproduction in any medium, provided the original author(s) and source are credited.
- Leonard D, Krishnamurthy M, Reaves CM, Denbaars SP, Petroff PM: Appl. Phys. Lett.. 1993, 63: 3203. COI number [1:CAS:528:DyaK2cXht1WrtbY%3D]; Bibcode number [1993ApPhL..63.3203L] COI number [1:CAS:528:DyaK2cXht1WrtbY%3D]; Bibcode number [1993ApPhL..63.3203L] 10.1063/1.110199View ArticleGoogle Scholar
- Bimberg D, Grundmann M, Ledentsov NN: Quantum Dot Heterostructures. Wiley, Chichester; 1999.Google Scholar
- Li S-S, Xia J-B, Liu J-L, Yang F-H, Niu Z-C, Feng S-L, Zheng H-Z: J. Appl. Phys.. 2001, 90: 6151. COI number [1:CAS:528:DC%2BD3MXoslKnurY%3D]; Bibcode number [2001JAP....90.6151L] COI number [1:CAS:528:DC%2BD3MXoslKnurY%3D]; Bibcode number [2001JAP....90.6151L] 10.1063/1.1416855View ArticleGoogle Scholar
- Pakarinen J, Polojärvi V, Aho A, Laukkanen P, Peng CS, Schramm A, Tukiainen A, Pessa M: Appl. Phys. Lett.. 2009, 94: 072105. Bibcode number [2009ApPhL..94g2105P] Bibcode number [2009ApPhL..94g2105P] 10.1063/1.3086298View ArticleGoogle Scholar
- Joyce BA, Jones TS, Belk JG: J. Vac. Sci. Technol. B. 1998, 16: 2373. COI number [1:CAS:528:DyaK1cXkvFSisLw%3D] COI number [1:CAS:528:DyaK1cXkvFSisLw%3D] 10.1116/1.590177View ArticleGoogle Scholar
- Wasserman D, Lyon SA, Hadjipanayi M, Maciel A, Ryan JF: Appl. Phys. Lett.. 2003, 83: 5050. COI number [1:CAS:528:DC%2BD3sXpvVejsLg%3D]; Bibcode number [2003ApPhL..83.5050W] COI number [1:CAS:528:DC%2BD3sXpvVejsLg%3D]; Bibcode number [2003ApPhL..83.5050W] 10.1063/1.1633683View ArticleGoogle Scholar
- Wasserman D, Lyon SA: Appl. Phys. Lett.. 2004, 85: 5352. COI number [1:CAS:528:DC%2BD2cXhtVCqs7bK]; Bibcode number [2004ApPhL..85.5352W] COI number [1:CAS:528:DC%2BD2cXhtVCqs7bK]; Bibcode number [2004ApPhL..85.5352W] 10.1063/1.1827351View ArticleGoogle Scholar
- Uccelli E, Bichler M, Nuernberger S, Abstreiter G, Fontcuberta i Morral A: Nanotechnology. 2008, 19: 045303. 10.1088/0957-4484/19/04/045303View ArticleGoogle Scholar
- Wen H, Wang ZM, Salamo GJ: Appl. Phys. Lett.. 2004, 84: 1756. COI number [1:CAS:528:DC%2BD2cXhvFCjt7s%3D]; Bibcode number [2004ApPhL..84.1756W] COI number [1:CAS:528:DC%2BD2cXhvFCjt7s%3D]; Bibcode number [2004ApPhL..84.1756W] 10.1063/1.1664018View ArticleGoogle Scholar
- Schmidbauer M, Seydmohamadi S, Grigoriev D, Wang ZhHM, Mazur YuI, Schafer P, Hanke M, Kohler R, Salamo GJ: Phys. Rev. Lett.. 2006, 96: 066108. COI number [1:STN:280:DC%2BD283gtVOlsg%3D%3D]; Bibcode number [2006PhRvL..96f6108S] COI number [1:STN:280:DC%2BD283gtVOlsg%3D%3D]; Bibcode number [2006PhRvL..96f6108S] 10.1103/PhysRevLett.96.066108View ArticleGoogle Scholar
- Liang BL, Wang ZhHM, Mazur YuI, Salamo GJ, DeCuir EA, Manasreh MO: Appl. Phys. Lett.. 2006, 89: 043125. Bibcode number [2006ApPhL..89d3125L] Bibcode number [2006ApPhL..89d3125L] 10.1063/1.2243865View ArticleGoogle Scholar
- Liang BL, Wang ZhHM, Mazur YuI, Seydmohamadi SH, Ware ME, Salamo GJ: Optics Express. 2007, 15: 8157. COI number [1:CAS:528:DC%2BD2sXht12gtrbM]; Bibcode number [2007OExpr..15.8157L] COI number [1:CAS:528:DC%2BD2sXht12gtrbM]; Bibcode number [2007OExpr..15.8157L] 10.1364/OE.15.008157View ArticleGoogle Scholar
- Xie Q, Madhukar A, Chen P, Kobayashi NP: Phys. Rev. Lett.. 1995, 75: 2542. COI number [1:CAS:528:DyaK2MXot1Oht7Y%3D]; Bibcode number [1995PhRvL..75.2542X] COI number [1:CAS:528:DyaK2MXot1Oht7Y%3D]; Bibcode number [1995PhRvL..75.2542X] 10.1103/PhysRevLett.75.2542View ArticleGoogle Scholar
- Solomon GS, Trezza JA, Marshall AF, Harris JJS: Phys. Rev. Lett.. 1996, 76: 952. COI number [1:CAS:528:DyaK28Xotl2htw%3D%3D]; Bibcode number [1996PhRvL..76..952S] COI number [1:CAS:528:DyaK28Xotl2htw%3D%3D]; Bibcode number [1996PhRvL..76..952S] 10.1103/PhysRevLett.76.952View ArticleGoogle Scholar
- Wang ZM, Shultz JL, Salamo GJ: Appl. Phys. Lett.. 2003, 83: 1749. COI number [1:CAS:528:DC%2BD3sXmvV2hs7g%3D]; Bibcode number [2003ApPhL..83.1749W] COI number [1:CAS:528:DC%2BD3sXmvV2hs7g%3D]; Bibcode number [2003ApPhL..83.1749W] 10.1063/1.1606891View ArticleGoogle Scholar